Vol. 16, No. 1, 2005 Solvent and Molecular Weight Effects on Fluorescence Emission of MEH-PPV 75
conjugated soluble electroluminescent polymers that the distribution of the effective conjugation length and,
combine the wide spectral emission range common to the consequently, the emission profile are changed. Moreover,
organic molecular compounds, with easy processability the conformations in solution are partially maintained in
and good mechanical properties. Solubility after deriva- the polymer films prepared from distinct solvents (memory
tization is due to the lowering of the interchain effect).22,23,33
interactions. One of the first soluble PPV derivatives, Here we report the systematic study of the concentration
reported in 1991 was poly(2-methoxy-5(2’-ethyl- on the photophysical properties of MEH-PPV films with
hexyloxy)-1,4-phenylenevinylene) (MEH-PPV) (Scheme three molecular weights in an attempt to describe the
1). 4,5 Since then, this polymer has been extensively evolution of the aggregation process. We have
explored regarding various aspects of its physical systematically studied the photophysical properties of MEH-
properties.6 One important aspect of the emission properties PPV films produced by solutions of different concentrations
of MEH-PPV is the assignment of its emissive centers. Apart to follow the sequential aggregation and to explain the
from the intrinsic chemical composition and macro- memory effect in films. Using two equally good solvents,
molecular architecture, the emission wavelength and we have attempted to explain why they were able to produce
electroluminescence efficiency depend on two main morphologically different films and why the differences
parameters: (i) the torsion angle of the conjugated found in solution persisted in the films of these MEH-PPV
backbone, which determines the conjugation length;7 (ii) samples. The criterion to select the solvents (chloroform
the occurrence of interchain interactions, leading to the and toluene) was the solubility parameter for MEH-PPV,
formation of excimers, aggregates, and/or polaron pairs which has been evaluated. Some physical characteristics of
(here we adopt the same definitions proposed by T-Q the solid state were also compared in order to correlate with
Nguyen et al.10 for excimers and aggregates in MEH-PPV the different molecular weights.
films: “a species in the electronic state, involving intra- or
inter-chains interactions, that modifies the fluorescence Experimental
spectrum and decrease true photoluminescence quantum
yield”). Electroluminescence efficiency of these species Materials
is depleted since they generate alternative pathways for
light emission due to energy or charge migration to non- Three MEH-PPV with different molar weights (and
radiative states.8-21 In addition, films processed by different polydispersities) were employed: M n = 51 kg mol -1
— — — — —
techniques are also morphologically different22,23 and (Mn / Mw = 8.8) (M51), Mn = 86 kg mol-1 (Mn / Mw = 4.9)
— — —
performance reproducibility requires further studies. (M86), Mn = 125 kg mol-1 (Mn / Mw = 5.2) (M125), all from
Sigma-Aldrich Chemical Co. They were used as received
(data from the supplier). Toluene and chloroform,
spectrophotometric grade from Acros, were also used as
received. Molecular weights ( Mn) were employed for
calculation of the molar concentration of all of the polymer
solutions, in units of mol L-1.
Photoluminescence studies of solutions of the MEH-
PPV with three molecular weights in toluene and
Scheme 1. Chemical structure of MEH-PPV.
chloroform were prepared in the concentration range from
Several studies with MEH-PPV are reported showing 10-8 mol L-1 to 10-4 mol L-1. Films were prepared by casting
the photoluminescence in solutions and in films prepared of the solutions in both solvents on a Petri dish, with slow
by distinct techniques (spin coating and casting from evaporation under a saturated solvent atmosphere, at room
solutions) in an attempt to understand the morphology of temperature, for 30 hours. Later, the films were dried in an
the films and to optimize the performance of the oven at a temperature of ca. 50 °C for 1 day. Film thicknesses
electroluminescent device.24-28 The role of the solvent were ca. 30-40 mm.
depends on its solvation power as a whole, as well as on its Small pieces of these films were also annealed at 70 °C
selectivity: it has been shown that some solvents, like THF for 5 min in an oven under dynamic vacuum to evaluate
and chloroform, have a preference for MEH-PPV possible morphological changes. This temperature is
ramifications, while others, like chlorobenzene, xylene and roughly at the glass transition, previously determined by
toluene, mainly solvate the polymer backbone, resulting DSC, but below the onset of the decomposition temperature
in different macromolecular conformations.8,29-32 This way, estimated by TGA under a non-oxidative atmosphere.
76 Cossiello et al. J. Braz. Chem. Soc.
Methods The solvents with the closest delta values to these were
toluene (8.9 cal1/2 cm3/2) and chloroform (9.3 cal1/2 cm3/2).36
We determined the crystallinity of the neat polymer Although we employed here only these two solvents, several
samples and of the films by X-ray diffraction using a model others were tested allowing us to classify: good solvents
XD-3A X-ray diffractrometer, with CuKa radiation, in the (nitrobenzene 10.0 cal1/2 cm3/2, o-xylene 8.8 cal1/2 cm3/2, carbon
range ca. 2° < 2θ < 50°, operating at 20 mA and 30 kV. tetrachloride 8.6 cal1/2 cm3/2, tetrahydrofuran 9.1 cal1/2 cm3/2),
Samples were supported on aluminum plates. The degree poor solvents (1,4-dioxane 10.0 cal1/2 cm3/2, ethyl acetate
of crystallinity was determined by deconvolution of the 9.1 cal1/2 cm3/2, tetrachloroethylene 9.3 cal1/2 cm3/2) and non-
diffraction peaks measured relative to the scattering band, solvents (n-hexane 7.3 cal1/2 cm3/2, n-heptane 7.4 cal1/2 cm3/2,
which defines the χRX value. methylcyclohexane 7.8 cal 1/2 cm 3/2, dimehyl sufoxide
Decomposition temperatures were determined by 12.0 cal1/2 cm3/2, acetronitrile 11.9 cal1/2 cm3/2, 2-ethyl hexanol
thermogravimetic analysis (TGA) under an argon 9.5 cal1/2 cm3/2)..
atmosphere (Thermogravimetric Analyzer Hi-Res, TA
Instruments, model 29500), performed at a heating rate of Results and Discussion
We also determined the glass transition by differential Characterization of the polymers
scanning calorimetry. DSC was performed using a DuPont
2910 differential scanning calorimeter (DSC) controlled X-ray diffraction of MEH-PPV shows some crystalline
by module 2000, calibrated with indium as standard, with peaks in pristine form that decrease in films (Figure 1a). The
a heating rate of 10 °C/min. Two runs were scanned: the value for a M125 pristine sample was ca. 5% while those for
first from room temperature to 170 °C, then the sample was M51 and M86, as well as for all films cast from their
cooled down at a rate of 20 °C/min to –150 °C and, heated solutions, were lower and could not be precisely determined
at the same rate to 170 °C. The glass transition temperatures
were determined using the data from the second heating
Fluorescence measurements were performed in a PC1TM
Photon Counting Spectrofluorimeter from ISS Inc.
Fluorescence spectra of polymer solutions and polymer
films were obtained. The polymer for these solutions was
dissolved under stirring, during several hours and then,
the solution was maintained in dark in a sealed flask. The
spectral range was from 360 to 500 nm for the excitation
spectra and from 500 to 700 nm for emission spectra. Slits
were selected for a spectral resolution of ±0.5 nm.
MEH-PPV solubility parameter
In order to select good solvents for MEH-PPV we
initially estimated its solubility parameter d (cal1/2 cm3/2)
since, to our knowledge, it has not been determined
experimentally. The method of group contribution35 was
used, according to:
where: δ is the solubility parameter, εco is the cohesive energy,
Fi stands for the contribution of each group in the repeating
unit and V for the molar volume. Using the values tabulated,35
the following values were found for d of MEH-PPV, Figure 1. X-ray diffraction spetra of M51, M86 and M125. Arrows
indicate the decrease of the molecular weight. a. pristine samples, b.
respectively: 9.1 cal1/2 cm3/2, 9.4 cal1/2 cm3/2 and 8.9 cal1/2 cm3/2. polymer films cast from toluene (---) or chloroform (—).
Vol. 16, No. 1, 2005 Solvent and Molecular Weight Effects on Fluorescence Emission of MEH-PPV 77
(Table 1). Although the crystallinity degrees for films
prepared by casting using both solvents are lower and can
not be precisely determined (they seem to be lower than
1%), the weak diffraction peaks are located in the same
diffraction angles in agreement with the orthorhombic
structure23 (Figure 1b). Compared to other reports, the
crystallinity is lower, probably due to the lower molecular
weight employed here. In addition, films of MEH-PPV
produced from chloroform solutions seem to exhibit lower
crystallinity than films from toluene solutions.
Table 1. Some physical properties of MEH-PPV having three dif-
ferent molecular weights
Mn/(kg mol-1) χRX (%) a
Td / °C b Tg / °C c
51 < 1% 217 and 401 53±5
86 < 1% 227 and 422 48±5
125 5 425 54±5
χRX is the crystallinity degree from the X-ray diffractogram; b Td is
the decomposition temperature from TGA at the peak maximum;
data from a DCS trace.
Decomposition temperatures were determined by
thermogravimetric analysis (TGA) (Table 1). Samples M86
and M51 undergo thermal decomposition in two steps (at
250 °C and at 380-400 °C) with a 10% mass loss in the first
Figure 3. DSC heating thermograms (10 °C/min) of MEH-PPV
step (Figure 2). On the other hand, MEH-PPV M125 M125 (---), M86 (—) and M51 (-∆-∆-) cast from chloroform (a)
degraded in a single step peaking at 427 °C. Since O2 and toluene (b).
enhances efficiency of the decomposition,37 to prevent or
at least minimize the thermal degradation, we performed crystallinity, no relevant transitions could be assigned to
the annealing processes at mild conditions (near the glass melting in the DSC curves.
transition) and under a dynamic vacuum.
Photoluminescence in dilute solutions
UV-Vis electronic absorption spectra of MEH-PPV
solutions show an intense absorption band at 490 nm (2.51
eV) whose peak position is practically independent of the
solvent. Absorbances of solutions with several
concentrations show a deviation from Lambert-Beer´s law
for concentrations greater than 10-6 mol L-1. Samples with
higher molecular weights are less soluble undergoing
deviations of the Beer-Lambert law at lower concentrations.
On the other hand, for dilute samples, the excitation band
peaked at 470 nm, which differs from the maximum of the
Steady-state fluorescence spectroscopy using three
Figure 2. Normalized mass loss and dm/dt curves from excitation wavelengths: at the blue-edge (λexc = 390 nm),
thermogravimetric analysis (TGA) for MEH-PPV M125 (---), M86 at the peak (λexc = 470 nm) and at the red-edge (λexc = 540
(____) and M51 (-∆-∆-).
nm) of the excitation band, was performed at several
The second DSC scan of MEH-PPV samples showed concentrations (from 10 -8 mol L-1 to 10-4 mol L-1), in
the glass transition temperature (Figure 3) in the range of solutions of toluene and chloroform as well as with films
ca. 60-70 °C. Although X-ray diffraction showed some of MEH-PPV.
78 Cossiello et al. J. Braz. Chem. Soc.
Figure 4 shows the excitation and fluorescence nm and 555 nm for MEH-PPV solutions in chloroform and
emission spectra of MEH-PPV, at the lowest concentration, toluene, respectively, independent of the molecular weights
10-8 mol L-1, in both solvents. As noted, the emission band and of the excitation wavelengths. The blue shift of
is virtually independent of the excitation wavelengths emission observed for the solvent with larger polarity
characteristic of the emission from an isolated excited state could, in principle, be interpreted by the larger
singlet intrachain exciton.10 Fluorescence peaks lie at 552 stabilization of the electronic ground state of the MEH-
Figure 4. Normalized fluorescence (λexc = 390 nm ---, λexc = 470 nm —, λexc = 540 nm -∆-∆-) and excitation (λem = 556 nm) spectra of MEH-PPV:
a., b. M51; c., d. M86 and e., f. M125, in toluene and chloroform respectively. Concentration 10-8 mol L-1.
Vol. 16, No. 1, 2005 Solvent and Molecular Weight Effects on Fluorescence Emission of MEH-PPV 79
PPV in comparison with the stabilization of the electronic
excited state.32,38 (3)
In addition, the excitation/absorption and the
fluorescence spectra are only roughly mirror images, which where: In is the intensity of the n manifold, Er is the
can be theoretically explained when the relative intensity geometrical relaxation energy and ν0 is the vibrational
of the first vibronic band is significantly enhanced in the frequency (cm-1).
fluorescence spectrum.39 The corresponding Stokes´s shifts, The geometrical relaxation energies are, 136 meV and
taken from the maxima of the excitation and of the 121 meV for chloroform and toluene solutions,
fluorescence spectra in toluene and chloroform are 3078 respectively. These values are slightly larger than those
cm-1 and 5401 cm-1, respectively. There are, some plausible reported for MEH-PPV blended with polyethylene, ca. 86
reasons for the difference of the Stokes´s shift in these two meV, which can be associated with the larger possibility of
solvents: (i) it is associated with the polymer/solvent relaxation in fluid solvents.42
interaction through the solvent´s optical parameters
(refractive index and dielectric constant); (ii) it is related
to the magnitude of the change of dipole moment of the
electronic ground state and the excited state; (iii) there are
some conformational changes induced by the solvent that
modify the effective conjugation lengths of the emitting
Figure 4 also shows that the emission band is broader
for the chloroform solution, which can be explained by
greater conformational disorder. It can be deconvoluted in
three vibronic bands (Figure 5) using the software Origin
version 6.0 with the spectrum in wavenumber scale and
fitting the peak profile with gaussian functions. For
comparison, the full width at the half maximum (FWHM)
of the 0-0 vibronic band (at 556 nm) for MEH-PPV M51
was determined by deconvolution with values of 1110
cm-1 and 1126 cm -1 for films spun from toluene and
chloroform, respectively. Although the deconvolution of
the spectra is always an arbitrary procedure because we
can choose the type of the functions (gaussian or
lorentizian or combined functions), we define the initial
values of FWHM and the maximum of the peaks, there is
no doubt that the relative intensities of the 0-0 and 0-1
bands are different for chloroform and toluene solutions.
Deconvolution results in three vibronic bands designated Figure 5. Normalized fluorescence spectra of MEH-PPV M86:
as 0-0 (556 nm), 0-1 (599 nm) and 0-2 (634 nm), whose (—) experimental curve, deconvoluted curves (---). Concentration:
10-8 mol L-1 in a. chloroform and b. toluene, λexc = 470 nm.
differences are approximately coincident with the
vibrational stretching modes of the C=C bonds. The relative Thus the higher intensity ratio for chloroform is
intensities of the 0-0 and 0-1 vibronic bands are taken attributed to the preferential solvation of the lateral groups
form the experimental curves, the solution in toluene (I0-0/ while toluene preferentially solvates the backbone.
I0-1 = 2.37) being distinct from that for chloroform (I0-0/I0-1 Moreover, the solvation layer formed by chloroform
= 2.09). Here I0-0 and I0-1 are the intensities taken at λem molecules surrounding the lateral groups tightens the
(0-0) = 556 nm and λem (0-1) = 594 nm, respectively. Taking polymer chain to maximize the solvent-moiety
these values, the Huang-Rhys parameter, S, (equation 2) interactions. Since the lateral groups can display several
and geometrical relaxation energy (equation 3) can be possible special orientations, several types of partially
determined.16 folded conformations can take place and, as a consequence,
the fluorescence spectra are broadened. Differently, toluene
and other aromatic solvents undergo preferential
(2) interaction with the conjugated polymer backbone
80 Cossiello et al. J. Braz. Chem. Soc.
(vinylene-phenylene groups), which adopt more planar are also similar to those obtained at 10-8 mol L-1 (data not
conformations. 7,9,10,14,21-23,26,28,32,43,44 One unequivocal shown). However, some evidence of preliminary
experimental demonstration of the preferential solvation aggregation of the polymer is revealed by the small change
of the lateral groups by non-aromatic solvents was the of the relative intensity of vibronic bands 0-0 and 0-1,
orientation of these groups perpendicular to the I0-0/I0-1, compared with that for the 10-8 mol L-1 solutions.
macromolecular back-bone making the film surface more For example, taking the experimental intensities at 556
polar whereas the coplanar orientation were observed when nm and 599 nm for MEH-PPV M86 in chloroform and
the film was spun using aromatic solvents.9 Consequently, toluene solutions we obtained I0-0/I0-1 = 1.89 and 1.92,
greater constraints are imposed on the backbone that limit respectively, which are lower than previously values (2.37
the possible number of conformations. More limited and 2.09). The aggregates of MEH-PPV emit at 600 nm in
distributions of conformers always lead to narrower coincidence with the vibronic 0-1 band of the intra-chain
fluorescence bands because the number of emissive Franck- isolated chromophore, which explains the relative increase
Condon (FC) states is more limited.34 of the intensity at 600 nm.26,30,33,40,41
In general, preferential solvation is analyzed in terms
of planarity instead of the solubility parameters or other
representations of polymer/solvent interactions. The
solubility parameters for toluene and chloroform are
relatively similar, 8.9 and 9.3 cal1/2 cm3/2, 36 respectively,
and, in principle, they could be equally good solvents for
MEH-PPV. However, their components are quite distinct:
although the dispersive components are very similar (δd =
8.82 and 8.65 cal 1/2 cm3/2 for toluene and choroform,
respectively) the polar components are distinct (δp = 0.7
and 1.5 cal 1/2 cm 3/2 for toluene and choroform,
respectively).36 In conclusion, although planarity can be
an important condition, specific interactions play an
important role for the preferential solvation, which is a
very complex phenomenon. The appropriateness of a
solvent can not be easily represented by a single solubility
parameter. Additional complexity is introduced when
solvents induce conformational changes of the conjugated
polymer chain that modify the effective lengths and the
size distribution of the conjugated emissive segments.
Consequently, the solvatochromism and the spectral profile
of the fluorescence and of the absorption band depend on
several factors: on the overlap of the vibronic progression,
on the configurational imperfections extrinsically imposed
by the solvent and intrinsically imposed by chemical Figure 6. Normalized fluorescence spectra of MEH-PPV M86 in a.
defects, on the configurational disorder, on the dynamics chloroform and b. toluene, with several concentrations: 10-8 mol L-1,
10-7 mol L-1, 10-6 mol L-1 and 10-5 mol L-1. Arrows indicate increase of
of polymer relaxation and on the dynamics of the concentration. λexc = 470 nm.
Figure 6 compares the fluorescence spectra of MEH-
Photoluminescence in concentrated solutions PPV M86 in solutions of several concentrations, from 10-8
to 10-5 mol L-1. Similar results were obtained for samples
Fluorescence spectra of MEH-PPV in more with other molecular weights and are omitted. Spectra of
concentrated solutions, 10-7 mol L-1 (Figure 6), are slightly toluene solutions are always sharper, the emissions of
red-shifted (2-3 nm) compared with the spectra of a 10-8 aggregates (λem = 600 nm) are relatively more intense,
mol L-1 solution (Figure 5). This red-shift is independent shifting the spectra to the red. Aggregates increase the
of the excitation wavelengths and is attributed to the inner- relative intensity of the 0-1 band because their emission is
filter effect, as often observed for concentrated solutions.34 red-shift compared with the isolated lumiphore are
The excitation spectra at the emission peak (557-560 nm) dimmers. If we assume that these aggregates are dimes and
Vol. 16, No. 1, 2005 Solvent and Molecular Weight Effects on Fluorescence Emission of MEH-PPV 81
that this red-shift originates from a exciton splitting,45 the independent of the excitation wavelengths (λexc = 390 nm,
expected value of the Davidov coupling is 2B ≅ 2500 cm-1, λexc = 470 nm and λexc = 540 nm), for toluene solutions the
which is in the range of the exciton splitting observed for lower intensity band at 598 nm has a higher intensity if
dimerization of small molecules46,47 and other conjugated the excitation takes place at the red-edge of the excitation
polymers.48 band, ca. λexc = 540 nm. In addition, there is a remarkable
As noted in Figure 7, the fluorescence emissions for decrease of the I0-0/I0-1 ratio, compared with the 10-8 mol L-1
solutions of 10-7 mol L-1 are also red-shifted compared solutions. This effect is much more pronounced for toluene
with the spectra of samples with lower concentration. solutions of M125.
Larger red-shifts occur for chloroform solutions of M125 As previously commented, the red-shift of the
(from 559 nm to 575 nm) compared to toluene (from 568 fluorescence spectra resulted from: (i) inner-filter effect
nm to 573 nm). Nevertheless, while for MEH-PPV in produced by the higher optical density of the more
chloroform the fluorescence emission is practically concentrated solutions; (ii) the conformational changes
Figure 7. Normalized fluorescence (λexc = 390 nm ---, λexc = 470 nm ___, λexc = 540 nm -∆-∆-) of MEH-PPV: a., b. M51; c., d. M86 and e., f. M125,
in toluene and chloroform respectively. Concentration 10-6 mol L-1.
82 Cossiello et al. J. Braz. Chem. Soc.
of the polymer chain that modify the effective size of the the blue-edge of the excitation band (λexc = 370 nm) leads
intra-chain conjugation; (iii) the formation of aggregates to the emission of higher energy specie, the isolated form,
that increases the relative intensity of the red-edge 0-1 while excitation at the red-edge (λ exc = 540 nm)
vibronic band (600 nm) and, (iv) interaction with the preferentially excites the lower energy aggregates that emit
solvent, producing solvatochromic effects. In principle, at the red-edge of the emission band. Although in toluene
the inner-filter effect depends only on the number of we observe site-selective excitation, in chloroform
chromophoric units present in solution, being independent solutions the emission is independent of the excitation
of the solvent (if differences of solubility are ignored).34 wavelengths even though the higher relative intensity of
Nevertheless, the inner-filter effect can not explain the the band at 600 nm evidenced the presence of aggregates.
simultaneous occurrence of: larger red-shift, higher Because of the difference in solvation ability and similar
intensity of the red-edge band (600 nm), higher vibronic to other reports, we assume that toluene undergoes a
resolution and stronger dependence of the spectral profile preferential solvation of the back-bone inducing a more
on the excitation wavelengths for toluene solutions of planar structure, which defines a sharper distribution of
M125. The more plausible reason for the larger changes conformations and sharper fluorescence emission bands.22
for M125 (compare Figure 7a,c, and e or 7b,d and f), is the Under this condition, site-selective emission can be
decrease of the solubility of longer chains. 37 The observed. On the other hand, preferential solvation of
enhancement of the intensity at 600 nm can be attributed lateral groups by chloroform leads to a more flexible back-
to, at least, two major reasons: aggregation of the polymer bone, several conformations are possible emission bands
chains in more concentrated solutions, principally when becomes broader and site-selective emission is not
the molecular weight increases, and changes of the observed. Although a precise explanation for these
conformational freedom. Nevertheless, there are several observations requires additional data, for example time-
reasons for our belief that aggregation predominates over resolved spectra, we suggest that in less ordered systems
the conformational disorder: (i) there is a relative increase additional energy transfer or migration processes occur
of the band at 600 nm where the emission of aggregates and the relative quantum efficiencies of the emission of
predominates; (ii) this relative intensity is more isolated and aggregate forms are maintained constant. On
pronounced for higher molecular weight samples, which contrary, successive energy transfer or migration was
one expects to be less soluble; (iv) there is a remarkable inhibited when a higher energy specie is preferentially
decrease of the entire intensity signal, which is compatible excited either because the radiative process is more
with the decrease of the quantum yield of aggregates efficient or because the lower energy specie (aggregate) is
compared to the isolated lumophores. On the other hand, inaccessible. In any case this point requires further studies.
increase of the conformational disorder should produce The red-shift of the absorption band is also observed in
different types of changes of the spectral profile, such as: (i) addition to the fluorescence spectra. This result can be
broadening of the emission band occurs when the interpreted according to the exciton theory developed by
conformational disorder increases; (ii) more flexible Kasha et al. 45 According to this model, the relative
conformations produce shorter conjugation lengths leading orientation of the transition moments of both interacting
to the blue-shift of the emission spectrum. Thus, considering molecules defines selection rules for electronic transitions
that none of these two behaviors were observed and of the dimer. For example, in the case of the anti-parallel
considering that the solubility decreases with the increase orientation of the transition moments, the allowed electronic
of the molecular weight, we conclude that the major reason transition is red-shifted compared to the isolated
for the relative increase of the intensity at 600 nm is the chromophores, as are the absorption/excitation bands. Based
aggregation of the polymer in concentrated solutions. on this simple model from the experimental data, we
Interaction with solvents with larger dipole moments conclude that, in concentrated solutions, an inter-
should shift the spectra to the blue or to the red, depending chromophoric interaction takes place with anti-parallel
on the stabilization of the electronic excited state.38,39 In orientation relative to the backbone of the two
particular some reports49 showed that there is a decrease of macromolecular segments.
the dipole moment for excited state MEH-PPV that should
result, as observed, in a blue shift of the fluorescence Photoluminescence of films
emission in more polar solvents.
Differences of the solvation abilities of chloroform and Here we show the fluorescence spectra of polymer films
toluene play an important role in controlling the shape of prepared by casting from dilute solutions (Figure 8). Film
the emission band. For toluene solution the excitation on thicknesses are very similar, ca. 30-40 µm. As previously
Vol. 16, No. 1, 2005 Solvent and Molecular Weight Effects on Fluorescence Emission of MEH-PPV 83
done for solutions, the analysis was carried out for both The site selective excitation of MEH-PPV films was
peak positions and the relative intensities of the vibronic performed at room temperature, which is below the glass
bands. Fluorescence spectra of all films are red-shifted and transition (Tg ≅ 60-70 °C) (Figure 2 and Table 1). Assuming
broader compared with concentrated solutions (Figure 7). that the polymer matrix is almost frozen below the glass
Better resolved vibronic bands are obtained for films cast transition and that the excitation of Franck-Condon (FC)
from toluene solutions, revealing a sharper distribution of states is a vertical process, preferential excitation and
macromolecular conformations. As observed before for emission take place when the decay is faster than the
toluene solutions the conformational disorder of the polymer relaxation processes.34,50,51 This assumption is
conjugated polymers in solution is partially retained in quite plausible for MEH-PPV since the fluorescence decays
the solid state (memory effect). occur in the range of hundreds of pico-seconds for the
Figure 8. Normalized fluorescence emission of films from chloroform (—) and toluene (---) of MEH-PPV M51 (a, b), M86 (c, d) and M125
(e, f). Right side: annealed samples.
84 Cossiello et al. J. Braz. Chem. Soc.
isolated chromophore and of a few nanoseconds for the volume,52,53 decreases the relative amount of larger free-
aggregates. 51 Under this assumption, the selective volumes, controls the polymer topology and produces
excitation with higher energy photons (λexc = 370 nm) of densification of the material.
smaller aggregates is responsible for the higher energy
emission (λem = 600 nm). On the contrary, photons with Conclusions
lower energy (λexc = 570 nm) excite larger aggregates that
emit with lower energy (λem = 630 nm). We have shown that two good solvents for MEH-PPV
As noted in Figure 8, while the wavelength range of (toluene and chloroform) undergo different interactions
the fluorescence emission (550-700 nm) is almost with the polymer, bringing about different conformations
independent of the excitation wavelengths regardless of in solution and cast films that are reflected in the
the molecular weights, the spectral profile depends on the photoluminescence properties.
excitation wavelengths, on the molecular weight and on Both solvents and the polymer molecular weights play
the solvent, as well. For example, excitation with lower important roles with respect to the photoluminescence
energy photons increases the relative intensity of the properties of MEH-PPV in solutions as well as in films.
emission at lower energy only for films cast from toluene. Annealing is an additional parameter to be controlled for
As pointed out, solvation in toluene induces a more planar films, since the conformational disorder in solutions is
conformation of the backbone, which favors the transferred to the solid-state. Even though we employed
aggregation in π,π-stacked inter-chain orientations, and two good solvents with comparable solubility parameters,
this effect is enhanced for M125 due to its lower their influences on film morphology and topology are
Films cast from chloroform solutions exhibit a broader A more extended conformation was maintained in films
spectrum (Figure 8), reflecting a broader distribution of cast from toluene, which enhances polymer aggregation.
conformers. They are more strongly affected by the Spectra of aggregates can be explained by the exciton
annealing at T ~ Tg. Their spectra become sharper, shifting splitting of the electronic levels according to Kasha’s
to the red and acquiring the same profile as those cast from model, where the orientation of the two chromophores is
toluene solutions. Topology of a sample of M86 was similar to the sandwich conformation of the excimer of
recorded by fluorescence optical microscopy at several aromatic molecules, leading to the formation of cofacial
temperatures. In Figure 9 some micrographs are shown (- p,p-stacked dimers.
100 °C, -50 °C, 50 °C and 100 °C). From these micrographs The concept of good solvents for MEH-PPV samples is
we observe that the corrugated topology at lower not easily correlated with the solubility parameters.
temperatures becomes flattened and more uniform at However, even when good solvents are employed, the
T ~ Tg. It is well known that annealing at T ~ Tg erases the observed micro-morphology of the solid state is not
thermal history of the samples, reduces the average free- necessarily the same. Molecular weights also play an
important role since the solubility decreases with the
increase of the molecular weight. Annealing at T ≅ Tg
stabilized the morphology of films prepared using different
solvents. This is a convenient temperature range to perform
the annealing process since it is enough to erase the thermal
history without significant polymer degradation.
Since the conformation in solution is partly retained
in the films, the solvent effects described can have an
important role in the electroluminescence properties of
this material, which is its most important application.
T.D.Z.A. and R.F.C. thank FAPESP, CNPq and MCT/
PADCT/IMMP for the financial support and a fellowships.
Figure 9. Optical fluorescence microscopy of films of MEH-PPV L.A. thanks CNPq for financial support and a fellowship.
M86 at several temperatures: a. –100 °C, b. –50 °C, c. 50 °C and d. The authors thank Prof. Carol Collins for useful
100 °C. Magnification is 50 times. Dimensional area: 910 µm x